A reinterpretation of the phase transitions in Na 2 CO 3


 Cecil Blaze Gray
 2 years ago
 Views:
Transcription
1 Acta Crystallographica Section B Structural Science ISSN Editor: Carolyn P. Brock A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva and Gervais Chapuis Copyright International Union of Crystallography Author(s) of this paper may load this reprint on their own web site provided that this cover page is retained. Republication of this article or its storage in electronic databases or the like is not permitted without prior permission in writing from the IUCr. Acta Cryst. (2005). B61, Arakcheeva and Chapuis Phase transitions in Na 2 CO 3
2 Acta Crystallographica Section B Structural Science ISSN A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva* and Gervais Chapuis Ecole Polytechnique Fédérale de Lausanne, Institut de Physique de la Matière Complexe, BSP, 1015 Lausanne, Switzerland Correspondence Based on the structural data of phases (hexagonal; K), (monoclinic; K), (incommensurate, monoclinic; 295 K) and (lockin, monoclinic; 110 K) of sodium carbonate, Na 2 CO 3, we could draw a parallel between the phase transitions and the evolution of the second coordination sphere of the C atoms. The temperaturedependent structures observed in the phase are reproduced in the incommensurate phase as a modulation wave, which relates to the content of the symmetrically equivalent {110} lattice planes in the phase. By decreasing the temperature, the phase transitions are associated with a stepwise increase in the number of Na ions participating in the second coordination sphere of the C atoms. Over the full temperature range, this number increases from 3 to 7. The C O distances and the mobility of the O atoms depends on the number of Na ions in the vicinity of the C atoms. Received 22 November 2004 Accepted 14 October 2005 # 2005 International Union of Crystallography Printed in Great Britain all rights reserved 1. Introduction Incommensurate structures are conveniently described in the superspace formalism. The obvious advantage is that their structures can recover lattice periodicity, in a space varying between four and six dimensions. If the incommensurate structure is part of a sequence of phases where both commensurate and incommensurate structures can exist, it appears that the theoretical tools are still incomplete in order to give a coherent view of the complete set of phases occurring at various temperatures or pressures. From the theoretical considerations of Parlinski & Chapuis (1993), the fundamental role of the atomic interactions of the second coordination sphere (cation cation for the anion containing compounds) was shown for the commensurate incommensurate phase transition. Based on the sequences of the temperaturedependent phases of Na 2 CO 3 (Fig. 1), we would like to illustrate this theoretical prediction and show that the specific cation cation interactions can be associated with each of the phase transitions which have been identified. In this context, the interaction must be understood in terms of the number of second nearestneighbour interactions which are characterized by distances smaller than a limiting distance which will be discussed later. The temperaturedependent phase transitions of Na 2 CO 3 have been widely studied (Wolff & Tuinstra, 1986; Harris & Salje, 1992; Swainson et al., 1995; Harris & Dove, 1995; Harris et al., 1996; Dušek et al., 2003). The following sequence of phases is supported by precise structural investigations which have been repeatedly confirmed: (i) : T = K; space group P6 3 =mmc; 10 refinements were reported by Swainson et al. (1995) for different temperatures; unitcell parameters: a = (2) Å and c Acta Cryst. (2005). B61, doi: /s
3 varies from to Å [the values a M = (4) and b M = Å refer to the monoclinic setting]. (ii) : T = K; space group C2/m; about 20 refinements were performed by Swainson et al. (1995) for different temperatures; unitcell parameters: a = 9.00 (2), b = 5.23 (2) Å, the c parameter and monoclinic angle vary from 6.21 to 6.44 Å and from 90 to 99.33, respectively. (iii) (incommensurate): T = K; superspace group C2/m (0)0s; the study was performed at 295 K (Dušek et al., 2003); unitcell parameters a = (7), b = (5), c = (5) Å, = (8), q = [0.182 (1), 0, (1)]. (iv) (lockin): T 170 K; space group P2 1 =n [equal to superspace group C2/m ( )0s]; the structural data were obtained at 110 K (Dušek et al., 2003); unitcell parameters a = (7), b = (5), c = (5) Å, = (8), q =[ 1 6, 0, 1 3 )]. In all the available publications, the phase transitions are associated with the tilt of the triangular CO 3 rigid units. However, their origins have been explained in two different ways. The! structure transformation was associated with a ferroelastic secondorder phase transition by Swainson et al. (1995), with the spontaneous shear strain (namely, the component 5 = acos =a 0 ) as the primary order parameter. In this model, the carbonate rotation simply follows rather than drives the shear strain. A lattice dynamics calculation based on a C O and Na O rigidbond model was invoked to justify this model. In Dušek et al. (2003), the origin of the! phase transition was associated with the tilting of the carbonate groups. The unsaturated bonding potential of the Na + ions was invoked in order to explain the progressive tilt of the CO 3 group. Indeed, the bondvalence sums (BVS) calculated by Dušek et al. (2003) demonstrate this tendency for one Na þ ion [BVS: 0.71 ()! 0.80 ()! 0.94 ()! 1.00 ()]. However, the other two Na þ ions become oversaturated with Na O bonds [BVS: 1.06 ()! 1.25 ()! 1.35 ()! 1.4 ()], which is not favorable for the structure stabilization. Hence, the question about the nature of the phase transitions is still open and the origin of the tilt of the CO 3 triangle at lower temperature remains without a plausible explanation. No evidence of any discontinuity at the transition temperatures was mentioned in any of the available publications dedicated to Na 2 CO 3 crystal structures. Only the C O and Na O interactions were considered in order to justify the transition mechanism. In the present article, we show that by decreasing the temperature some dramatic changes occur in this structure between nono atoms, which are associated with the phase transformations. Based on an analysis of the structural data obtained from Swainson et al. (1995) and Dušek et al. (2003) for all modifications mentioned above, we postulate that the gradual strengthening of the C Na interactions (decrease of C Na distances from 3.4 to Å) is the main structural feature underlying all the phase transitions observed over decreasing temperatures. All the temperaturedependent Figure 1 The crystal structure of Na 2 CO 3 :(a) perspective view and (b) the (001) projection. The Na3 and [CO 3 ] ions form graphitelike layers, parallel to (001) and stacked in the third direction. The Na1,2 ions are located in the hexagonal channels. The three atomic planes of the {110} hex family contain all the atoms of the structure. They are equivalent in the hexagonal phase and indicated as m M and m V corresponding to one mirror plane and two virtual mirror planes in the monoclinic modifications. The monoclinic unit cell is shown with a dashed line. Figure 2 Temperature dependence of the C Na distances in the K range. Various dots and solid lines indicate the experimental data published in Swainson et al. (1995) and Dušek et al. (2003). The solid vertical lines correspond to the phase transition temperatures. The gray areas indicate modulated distances and the doublesided arrows indicate the antiphase modulations in the two m V planes. The dashed lines are approximations. The incommensurate 0 phase is derived from a reinterpretation of the experimental data. 602 Arakcheeva and Chapuis Phase transitions in Na 2 CO 3 Acta Cryst. (2005). B61,
4 transformations, such as the increase of the monoclinic angle (justifying the 5 = a cos */a 0 shear strain component), the tilt of the CO 3 triangles, the difference between the O1 and O2 atomic displacements and the C O distances, follow directly from the decrease of the C Na distances on decreasing the temperature. The result is a stepwise formation of C Na bonds, i.e. C Na distances shorter than 3.1 Å. [It is worth mentioning that the C Na distances, Å, characteristic of oxygenfree Na 2 C 2 (Hemmersbach et al., 1999) are close to these values.] We show that each successive phase transition is correlated with the formation of an additional bond in the second coordination sphere of C atoms. The C Na bond formation is not continuous at the! transition temperature. The! transformation mechanism is more complex than the description given in Swainson et al. (1995). From the experimental data, our analysis allows the prediction and confirmation of the existence of an additional modification of the incommensurate phase. channel atoms, the other corresponding to the interlayer C Na3 distance. Both distances are located on a series of atomic planes parallel to {110} hex (Fig. 1). In the hexagonal phase, these atomic planes correspond to the mirror planes m. In the monoclinic modifications, only one of the planes, namely m M (Fig. 1), remains as a mirror plane. In this context, the other two are called m V (virtual mirror) planes (Fig. 1). Our analysis (Fig. 2) of the structural data shows that the series of phase transitions observed by decreasing temperature is associated with the formation of C Na bonds in the family of {110} hex atomic planes. The first step is the formation of bonds in the monoclinic m M mirror plane. The second step is the formation of C Na bonds in the two m V planes of the incommensurate phase: two antiphase waves of the C Na distances appear respectively in two m V planes along the internal t axis. The analogy of the temperature dependence 2. The phase transitions and the C Na bond formation The structure of Na 2 CO 3 (Fig. 1) can be described as graphitelike layers formed by Na3 and CO 3 ions, which are stacked along the hexagonal axis. Additional Na1,2 ions are located in the hexagonal channels. The graphitelike layers are regular in all modifications and all the C Na3 bonds are characterized by the minimum temperatureindependent distances, Å (Fig. 2). The two other types of C Na distances found in the hexagonal hightemperature phase are longer ( 3.4 Å), pointing to weak interactions. One of them corresponds to the C Na1,2 distance between the layer and Figure 3 Analogy of the modulation wave and the temperature dependence in the {110} hex family of planes. Interatomic distances smaller than 3.1 Å are shown by solid lines. The temperaturedependent evolution of the C Na2 distance, Na3 C Na3 angle and O2 displacement in the m M plane in the phase (left). Following the modulation along t, the same types of magnitudes occur again for C Na1, Na3 C Na3 angle and O1 displacement in the m V plane along c in the phase (right). Figure 4 Phase transition scheme of Na 2 CO 3. The structural transformations take place in the family of atomic planes {110} hex. In the phase the interlayer C Na3 distance decreases from 3.35 (972 K) to 3.23 Å (754 K). In the phase significant changes appear on the mirror m M plane: the decrease in the C Na2 distances from 3.4 to 3.18 Å and C Na3 from 3.23 to 3.1 Å induces an increase of the monoclinic angle from 90 (754 K) to (605 K); the decrease in the C Na2 distance is associated with a shift of O2. In the phase significant transformations appear in the two m V planes as antiphase modes along t: the C Na1 distances vary between 3.4 and 3.0 Å; the decrease of the C Na1 distance is associated with a shift of O1. In the phase the content of the m M plane is slightly affected by temperature: the monoclinic angle changes only by 2.5 between 605 and 110 K; the convergence of the C Na3 and C Na2 distances also induces a convergence in the O2 atomic position. Acta Cryst. (2005). B61, Arakcheeva and Chapuis Phase transitions in Na 2 CO 3 603
5 and the modulation wave of the C Na distances in the planes of the {110} hex family is illustrated in Fig. 3. This analogy confirms the common nature of the C Na interactions and points to a unique mechanism, inducing the sequence of phase transitions. The structural transformation scheme is described in Fig. 4. A few remarkable features extracted from the distance temperature diagrams of Fig. 2 should be underlined in this context. (i) At the! transition, which occurs at 754 K, the interlayer distance C Na3 = 3.23 Å splits into two distances, 3.1 and 3.35 Å, indicating a discontinuity in the structural transformation. (ii) The shortest value matches the bond range and does not vary in the temperature range of the phase. Another value reaches the bond range close to the! transition temperature of 605 K. At this temperature, the interlayer distance splits once more, varying from 3.1 to 2.9 Å along the internal t axis in the phase. This splitting again indicates a discontinuity of the structural transformation at 605 K. (iii) In the temperature range of phase the variation in the C Na3 interlayer distances is independent of the continuously decreasing C Na2 distance, which causes the intensive increase of the monoclinic angle in the m M plane (Fig. 4) that justifies the 5 = acos =a 0 shear strain component. (iv) This C Na2 distance (3.18 Å at the transition temperature of 605 K) can still decrease in order to form a bond. This distance decreases continuously, reaching the bond value 3.1 Å only at 530 K (Fig. 2). At this temperature we can expect the splitting of the C Na1 distance by antiphase modulations in the m V atomic planes. This occurs only after the formation of all the possible C Na bonds in the m M atomic plane. Therefore, we propose an additional phase transformation at 530 K: incommensurate 0 incommensurate. This is confirmed by the experimental Xray diffraction pattern relating to the thermal treatment and the temperature dependence of the component of the q vector, both published in de Wolff & Tuinstra (1986); Figs. 1 and 7, respectively. The IR spectra of the CO 3 group discussed below are also compatible with this assumption. The temperaturedependent modulation vector q becomes rational, q = 1 6 a þ 1 3 c, at the to transition. At this temperature, the commensurate ordering of the C Na bonds results in a multiple monoclinic unit cell. In the lockin phase, the antiphase modulation of the C Na1 distances observed in the incommensurate phase freezes, resulting in three short (< 3.14 Å) and three long (> 3.29 Å) distances at 110 K. It can be expected that by further decreasing the temperature, the three shorter C Na1 distances in the phase will reach the shortest possible bond distances of Å. The evolution of the C Na3 and C Na1,2 distances is associated with the corresponding evolution of the Na1 Na2 and Na3 Na1,2 distances, as seen in Figs. 3 and 4. However, in contrast to the C Na distances, the Na Na distances decrease smoothly from 3.4 to 3.0 Å and do not show any specific characteristic of a phase transition. Figure 5 Evolution of the Na environment in the vicinity of the C atom. The coordination number (CN) of the C atom is limited to the C Na distances of up to 3.1 Å. The projections of [CNa n ] polyhedra are plotted in two different planes of the {110} hex family. Nonbonded Na ions are shown by circles. The environment of the C atom including both Na ions and O atoms is also presented (center). Figure 6 tdependence of the C Na distances in the vicinity of the C atom in the (lines) and (dots) phases. Six Na ions are always present in the second coordination sphere of C within the 3.1 Å radius (gray area). The bold line indicates the modulation of the seventh Na ion in the vicinity of C in the phase. 604 Arakcheeva and Chapuis Phase transitions in Na 2 CO 3 Acta Cryst. (2005). B61,
6 3. The Na environment of the C atom and the phase transition The formation of the C Na bonds which gradually appear on decreasing the temperature are associated with an increase in the number of Na ions in the vicinity of the C atoms, i.e. the coordination number (CN) of C in the second coordination sphere. In Fig. 5 the temperaturedependent evolution of the Na environment of the C atom within the 3.1 Å is projected on the m M and m V planes. Fig. 5 also indicates an increase in the plane density on decreasing the temperature. It is significant that every additional bond formation (the increase of CN by 1) always relates to a new phase transition (Fig. 5, center). The three Na ions surrounding the C atom on the graphitelike layer correspond to CN = 3 in the phase. At 754 K, the! transition is characterized by a change of coordination number from 3 to 4 owing to the splitting of the interlayer C Na3 distance. The! 0 transition temperature at 605 K increases the CN to 5. At 530 K, the 0! transition temperature, the CN increases to 6 owing to the formation of the C Na2 bonds in the m M atomic plane. An antiphase modulation of two C Na1 distances located on two m V atomic planes appears at this temperature, thus producing domains of CN = 6 and a smaller fraction with CN = 7 in the incommensurate phase. The change in CN along the internal taxis can be extracted from Fig. 6. At the! transition temperature, 170 K, the periodic sequence of CN (6, 6, 7) is realised once the modulation vector q reaches [1/6, 0, 1/3] (Fig. 6). A complete stabilization of CN = 7 in the phase can only be reached at lower temperature. From this description, it can be concluded that in Na 2 CO 3 and by deceasing the temperature, the phase transitions are characterized by an increase of the number of C Na bonds (respectively CN) in the second coordination sphere of the C atoms. Knowing that the intralayer bonds are constant over the whole temperature range, this number increases owing to the strengthening of both interlayer C Na3 interactions and interactions between the layers and the channel atoms, Na1 and Na2. None of the channel atoms are bonded in the phase, whereas they are completely bonded to the C atom in the lowest phase. Taking into account the crystallographic analogy between C and Na3 (Fig. 1), we can state that the phase transitions are linked to an increase in the nono atom concentration close to the intersections of the most densely packed atomic planes, namely the graphitelike layers [the (001) planes] and the three planes of the {110} hex family. Both C and Na3 are located at these intersections. At each intersection and within 3.1 Å, the nonoatom concentration increases on decreasing the temperature: in the graphitelike layer of the phase ( K) only one atom can be found within this radius. In the phase ( K) the number increases to two owing to the interlayer contacts. The concentration increases from 2 to 2.5 Figure 7 Correlation between the temperature dependences of the C O distances (dots and lines) and the numbers of Na ions (CN) in the second coordination sphere (R = 3.1 Å) of the C atom. Dashed lines are approximations. The C O2 and C O1 distances are located on the m M respectively m V planes. The distances are given without a libration correction. Figure 8 Correlation between the first (O atoms) and the second (Na ions) coordination spheres of C in the and phases. Acta Cryst. (2005). B61, Arakcheeva and Chapuis Phase transitions in Na 2 CO 3 605
7 atoms, which corresponds to the progressive deformation of the atomic arrangement on the m M plane of the 0 phase ( K). A modulation of the concentration from 2.5 to 3 atoms appears in the phase owing to the atomic arrangement on the m V planes ( K). At 110 K, the phase, we find an ordered sequence of atom concentration (2.5, 2.5, 3) aligned along q. We postulate a value of 3 for the atom concentration as a limiting value at the lowest temperature of the phase. 4. Influence of the Na environment on the CO 3 group The temperature dependence of the Na environment of the C atom is correlated to both a tilt of the CO 3 group (Fig. 5) and the C O distances (Fig. 7). This correlation is illustrated in Fig. 8. The O atoms attempt to avoid the screening for the C Na interactions. This is why the O atom deviates gradually from the C Na line in the corresponding plane (Fig. 3 5 and 8). As a consequence, we observe a tilt of the CO 3 triangle. As can be deduced from Fig. 8, the increase of the C Na bond number and the associated decrease of the bond length induces an increase of the C O distances in the family of atomic planes {110} hex (Fig. 7). Therefore, the difference between the C O1 (in m V ) and C O2 (in m M ) distances, the very large anisotropy of their thermal libration (discussed by Wolff & Tuinstra, 1986, for and phases), and the difference in the tdependent displacements between O1 and O2 revealed by Dušek et al. (2003) are a direct consequence of the lengths and numbers of C Na bonds. In other words, the carbonate group is not a fully rigid unit. Moreover, the complex IR absorption spectra of the internal modes of the carbonate ion revealed in Harris & Salje (1992) are also directly correlated with the CN of the C atom (Fig. 5 and 9). 5. Conclusions We have established a direct link between the C Na distances and the sequence of phase transformations in Na 2 CO 3, which is systematic over the full range of phases. By decreasing the temperature, the consecutive increase of the C Na bond number (CN) in the second coordination sphere of the C atom as 3! 4! 5! 6 7! 7 fits respectively the!! 0 (predicted)!! phase transitions. This is the main conclusion of the present work. Consequently, we propose to directly associate the C Na bond formation with the phase transition mechanism: (i) The! phase transition which appears at 754 K is characterized by a splitting of the C Na3 = 3.23 Å interlayer distance ( phase) into 3.1 and 3.35 Å ( phase). This splitting clearly defines the internal structure discontinuity, but does not affect the lattice parameters and, therefore, cannot be characterized by or be caused by any spontaneous shear strain, including 5 discussed by Swainson et al. (1995) for Na 2 CO 3 as the primary order parameter of the secondorder ferroelastic! phase transition. However, this interlayer C Na3 bond formation can be a reason for the widely discussed lattice melting observed at the phase transition (Swainson et al., 1995; Harris & Dove, 1995, Harris et al., 1996). Therefore, the! phase transition needs a more consistent interpretation. (ii) The! 0 transformation is a firstorder phase transition of the commensurate incommensurate type at 605 K. The appearance of modulations affects the interlayer C Na3 distances; no significant modulation of the C Na1 distances can be observed. (iii) We propose a new incommensurate incommensurate phase transition, 0! at 530 K. This transition is associated with the creation of a highamplitude antiphase modulation of C Na1 distance in two planes of the (110) hex family. (iv) The! incommensurate lockin transformation is related to the ordering of the C Na1 bonds in threedimensional space. This work is supported by the Swiss National Science Foundation, grant Nos and M. Dušek is also gratefully acknowledged for his kind help. Figure 9 Correlation between the IR spectra of the CO 3 internal modes (after Harris & Salje, 1992) and the Na environment of the C atom at different temperatures. The solid vertical lines correspond to the phasetransition temperatures. References Dušek, M., Chapuis, G., Meyer, M. & Petřìček, V. (2003). Acta Cryst. B59, Harris, M. J. & Dove, M. T. (1995). Modern Phys. Lett. B, 9, Harris, M. J., Dove, M. T. & Godfrey, K. W. (1996). J. Phys. Condens. Matter, 8, Arakcheeva and Chapuis Phase transitions in Na 2 CO 3 Acta Cryst. (2005). B61,
8 Harris, M. J. & Salje, K. H. (1992). J. Phys. Condens. Matter, 4, Hemmersbach, S., Zibrowius, B. & Ruschewitz, U. (1999). Z. Anorg. Allg. Chem. 625, Parlinski, K. & Chapuis, G. (1993). Phys. Rev. B, 47, Swainson, I. P., Dove, M. T. & Harris, M. J. (1995). J. Phys. Condens. Matter, 7, Wolff, P. M. & Tuinstra, F. (1986). Incommensurate Phases in Dielectrics, edited by R. Blinc & A. P. Levanyuk, Vol. 2, pp Amsterdam: NorthHollandElsevier. Acta Cryst. (2005). B61, Arakcheeva and Chapuis Phase transitions in Na 2 CO 3 607
Plate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationPublication of smallunitcell structures in Acta Crystallographica Michael Hoyland ECM28 University of Warwick, 2013
Publication of smallunitcell structures in Acta Crystallographica Michael Hoyland ECM28 University of Warwick, 2013 International Union of Crystallography 5 Abbey Square Chester CH1 2HU UK International
More informationThe Crystal Structures of Solids
The Crystal Structures of Solids Crystals of pure substances can be analyzed using Xray diffraction methods to provide valuable information. The type and strength of intramolecular forces, density, molar
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationXRay Diffraction. wavelength Electric field of light
Light is composed of electromagnetic radiation with an electric component that modulates versus time perpendicular to the direction it is travelling (the magnetic component is also perpendicular to the
More informationAb initio structure solution from electron precession data by charge flipping. Lukas Palatinus. Institute of Physics AS CR, Prague
Ab initio structure solution from electron precession data by charge flipping Lukas Palatinus Institute of Physics AS CR, Prague What is charge flipping? Charge flipping is a method for ab initio determination
More informationChem 106 Thursday Feb. 3, 2011
Chem 106 Thursday Feb. 3, 2011 Chapter 13: The Chemistry of Solids Phase Diagrams  (no BornHaber cycle) 2/3/2011 1 Approx surface area (Å 2 ) 253 258 Which C 5 H 12 alkane do you think has the highest
More informationCapacitance and Ferroelectrics
Ram Seshadri MRL 2031, x6129 seshadri@mrl.ucsb.edu; http://www.mrl.ucsb.edu/ seshadri/teach.html Capacitance and Ferroelectrics A voltage V applied across a capacitor of caacitance C allows a quantity
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationMolecular Dynamics Simulations
Molecular Dynamics Simulations Yaoquan Tu Division of Theoretical Chemistry and Biology, Royal Institute of Technology (KTH) 201106 1 Outline I. Introduction II. Molecular Mechanics Force Field III. Molecular
More informationStructure Factors 59553 78
78 Structure Factors Until now, we have only typically considered reflections arising from planes in a hypothetical lattice containing one atom in the asymmetric unit. In practice we will generally deal
More informationCoordination and Pauling's Rules
Page 1 of 8 EENS 2110 Tulane University Mineralogy Prof. Stephen A. Nelson Coordination and Pauling's Rules This document last updated on 24Sep2013 The arrangement of atoms in a crystal structure not
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationMartensite in Steels
Materials Science & Metallurgy http://www.msm.cam.ac.uk/phasetrans/2002/martensite.html H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used
More informationCrystal Structure Determination I
Crystal Structure Determination I Dr. Falak Sher Pakistan Institute of Engineering and Applied Sciences National Workshop on Crystal Structure Determination using Powder XRD, organized by the Khwarzimic
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationphys4.17 Page 1  under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon
Covalent Crystals  covalent bonding by shared electrons in common orbitals (as in molecules)  covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationThe Unshifted AtomA Simpler Method of Deriving Vibrational Modes of Molecular Symmetries
Est. 1984 ORIENTAL JOURNAL OF CHEMISTRY An International Open Free Access, Peer Reviewed Research Journal www.orientjchem.org ISSN: 0970020 X CODEN: OJCHEG 2012, Vol. 28, No. (1): Pg. 189202 The Unshifted
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More informationIonic Bonding Pauling s Rules and the Bond Valence Method
Ionic Bonding Pauling s Rules and the Bond Valence Method Chemistry 754 Solid State Chemistry Dr. Patrick Woodward Lecture #14 Pauling Rules for Ionic Structures Linus Pauling,, J. Amer. Chem. Soc. 51,,
More informationAnharmonicity and Weak Mode Assignment in La 2 x Sr x CuO 4 with Oxygen Isotopic Substitution
Vol. 111 (2007) ACTA PHYSICA POLONICA A No. 1 Proceedings of the Symposium K: Complex Oxide Materials for New Technologies of EMRS Fall Meeting 2006, Warsaw, September 4 8, 2006 Anharmonicity and Weak
More information11.1. Objectives. Component Form of a Vector. Component Form of a Vector. Component Form of a Vector. Vectors and the Geometry of Space
11 Vectors and the Geometry of Space 11.1 Vectors in the Plane Copyright Cengage Learning. All rights reserved. Copyright Cengage Learning. All rights reserved. 2 Objectives! Write the component form of
More informationJournal of the University of Chemical Technology and Metallurgy, 42, 2, 2007. 2) are in C 1
Journal of the University of Chemical M. Georgiev, Technology D. Stoilova and Metallurgy, 42, 2, 2007, 211216 METALWATER INTERACTINS AND HYDRGEN BND STRENGTH M. Georgiev 1, D. Stoilova 2 1 University
More informationXray Powder Diffraction Pattern Indexing for Pharmaceutical Applications
The published version of this manuscript may be found at the following webpage: http://www.pharmtech.com/pharmtech/peerreviewed+research/xraypowderdiffractionpatternindexingfor Phar/ArticleStandard/Article/detail/800851
More informationBCM 6200  Protein crystallography  I. Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS
BCM 6200  Protein crystallography  I Crystal symmetry Xray diffraction Protein crystallization Xray sources SAXS Elastic Xray Scattering From classical electrodynamics, the electric field of the electromagnetic
More informationNo Evidence for a new phase of dense hydrogen above 325 GPa
1 No Evidence for a new phase of dense hydrogen above 325 GPa Ranga P. Dias, Ori Noked, and Isaac F. Silvera Lyman Laboratory of Physics, Harvard University, Cambridge MA, 02138 In recent years there has
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More informationGuide to Understanding Xray Crystallography
Guide to Understanding Xray Crystallography What is Xray Crystallography and why do I need to learn it? Xray Crystallography is a scientific method of determining the precise positions/arrangements
More informationNuclear reactions determine element abundance. Is the earth homogeneous though? Is the solar system?? Is the universe???
Nuclear reactions determine element abundance Is the earth homogeneous though? Is the solar system?? Is the universe??? Earth = anion balls with cations in the spaces View of the earth as a system of anions
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationInfrared Spectroscopy: Theory
u Chapter 15 Infrared Spectroscopy: Theory An important tool of the organic chemist is Infrared Spectroscopy, or IR. IR spectra are acquired on a special instrument, called an IR spectrometer. IR is used
More informationPhase determination methods in macromolecular X ray Crystallography
Phase determination methods in macromolecular X ray Crystallography Importance of protein structure determination: Proteins are the life machinery and are very essential for the various functions in the
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationBENTONITEMETHYLAMINE COMPLEXES i
BENTONITEMETHYLAMINE COMPLEXES i by I~ICKiRDS A. ROWLAND ~ AND E. JOSEPH WEISS a Shell Development Company (A Division of Shell Off Company), Exploration and Production Research Division, Houston, Texas
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationCHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS
CHAPTER THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts.6 Show that the atomic packing factor for HCP is 0.74. The APF is just the total sphere volumeunit cell volume ratio.
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationSolid State Device Fundamentals
Solid State Device Fundamentals ENS 345 Lecture Course by Alexander M. Zaitsev alexander.zaitsev@csi.cuny.edu Tel: 718 982 2812 Office 4N101b 1 Solids Three types of solids, classified according to atomic
More informationChapter 13 The Chemistry of Solids
Chapter 13 The Chemistry of Solids Jeffrey Mack California State University, Sacramento Metallic & Ionic Solids Crystal Lattices Regular 3D arrangements of equivalent LATTICE POINTS in space. Lattice
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationKEANSBURG SCHOOL DISTRICT KEANSBURG HIGH SCHOOL Mathematics Department. HSPA 10 Curriculum. September 2007
KEANSBURG HIGH SCHOOL Mathematics Department HSPA 10 Curriculum September 2007 Written by: Karen Egan Mathematics Supervisor: Ann Gagliardi 7 days Sample and Display Data (Chapter 1 pp. 447) Surveys and
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationChapter 3: Structure of Metals and Ceramics. Chapter 3: Structure of Metals and Ceramics. Learning Objective
Chapter 3: Structure of Metals and Ceramics Chapter 3: Structure of Metals and Ceramics Goals Define basic terms and give examples of each: Lattice Basis Atoms (Decorations or Motifs) Crystal Structure
More informationCHAPTER FIVE. 5. Equations of Lines in R 3
118 CHAPTER FIVE 5. Equations of Lines in R 3 In this chapter it is going to be very important to distinguish clearly between points and vectors. Frequently in the past the distinction has only been a
More information* Dr. Jyotsna Chauhan, * Dr. Rachna Tiwari, ** Dr. R.K Tiwari
Comparative XRay Structure analysis of systemic fungicides (N(2,6 dimethyl phenyl)n(2keto1 methyl butyl) 3hydroxypropanamide) AND cis N(1,1,2,2tetrachloroethylthio)4cyclohexene1,2 dicarboximide)
More informationThe nearlyfree electron model
Handout 3 The nearlyfree electron model 3.1 Introduction Having derived Bloch s theorem we are now at a stage where we can start introducing the concept of bandstructure. When someone refers to the bandstructure
More informationFigure 1.1 Vector A and Vector F
CHAPTER I VECTOR QUANTITIES Quantities are anything which can be measured, and stated with number. Quantities in physics are divided into two types; scalar and vector quantities. Scalar quantities have
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationCommunicated March 31, 1951 CHR CHR CHR. *H* zz '" *H _ 0....H / k C,.. CHR CNR CHR CHR CHR *HN/' N 'H_N/' H_./  H(H.
VOL. 37, 1951 CHEMISTR Y: PA ULING AND COREY 251 THE PLEATED SHEET, A NEW LAYER CONFIGURATION OF POL YPEPTIDE CHAINS BY LINUS PAULING AND ROBERT B. COREY GATES AND CRELLIN LABORATORIES OF CHEMISTRY,* CALIFORNIA
More informationModification of PdH 2 and PdD 2 thin films processed by HeNe laser
Modification of PdH 2 and PdD 2 thin films processed by HeNe laser V.Nassisi #, G.Caretto #, A. Lorusso #, D.Manno %, L.Famà %, G.Buccolieri %, A.Buccolieri %, U.Mastromatteo* # Laboratory of Applied
More informationStructural Axial, Shear and Bending Moments
Structural Axial, Shear and Bending Moments Positive Internal Forces Acting Recall from mechanics of materials that the internal forces P (generic axial), V (shear) and M (moment) represent resultants
More informationNEW MEXICO Grade 6 MATHEMATICS STANDARDS
PROCESS STANDARDS To help New Mexico students achieve the Content Standards enumerated below, teachers are encouraged to base instruction on the following Process Standards: Problem Solving Build new mathematical
More informationRay Optics Minicourse COMSOL Tokyo Conference 2014
Ray Optics Minicourse COMSOL Tokyo Conference 2014 What is the Ray Optics Module? Addon to COMSOL Multiphysics Can be combined with any other COMSOL Multiphysics Module Includes one physics interface,
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationAlgebra 2 Chapter 1 Vocabulary. identity  A statement that equates two equivalent expressions.
Chapter 1 Vocabulary identity  A statement that equates two equivalent expressions. verbal model A word equation that represents a reallife problem. algebraic expression  An expression with variables.
More informationBiggar High School Mathematics Department. National 5 Learning Intentions & Success Criteria: Assessing My Progress
Biggar High School Mathematics Department National 5 Learning Intentions & Success Criteria: Assessing My Progress Expressions & Formulae Topic Learning Intention Success Criteria I understand this Approximation
More informationElastic properties of orientationally disordered crystal of mono and polydisperse hard dumbbells in three dimensions
Materials SciencePoland, Vol. 26, No. 4, 2008 Elastic properties of orientationally disordered crystal of mono and polydisperse hard dumbbells in three dimensions M. KOWALIK, K.W. WOJCIECHOWSKI * Institute
More informationXray, DTA and Raman studies of monoclinic tridymite and its higher temperature orthorhombic modification with varying temperature
Journal of Mineralogical and Petrological Sciences, Volume 100, page 55 69, 2005 Xray, DTA and Raman studies of monoclinic tridymite and its higher temperature orthorhombic modification with varying temperature
More informationExploring Spherical Geometry
Exploring Spherical Geometry Introduction The study of plane Euclidean geometry usually begins with segments and lines. In this investigation, you will explore analogous objects on the surface of a sphere,
More information1.3. DOT PRODUCT 19. 6. If θ is the angle (between 0 and π) between two nonzero vectors u and v,
1.3. DOT PRODUCT 19 1.3 Dot Product 1.3.1 Definitions and Properties The dot product is the first way to multiply two vectors. The definition we will give below may appear arbitrary. But it is not. It
More informationCHAPTER 6 Chemical Bonding
CHAPTER 6 Chemical Bonding SECTION 1 Introduction to Chemical Bonding OBJECTIVES 1. Define Chemical bond. 2. Explain why most atoms form chemical bonds. 3. Describe ionic and covalent bonding.. 4. Explain
More informationSection 1.1. Introduction to R n
The Calculus of Functions of Several Variables Section. Introduction to R n Calculus is the study of functional relationships and how related quantities change with each other. In your first exposure to
More informationChapter 3. 1. 3 types of materials amorphous, crystalline, and polycrystalline. 5. Same as #3 for the ceramic and diamond crystal structures.
Chapter Highlights: Notes: 1. types of materials amorphous, crystalline, and polycrystalline.. Understand the meaning of crystallinity, which refers to a regular lattice based on a repeating unit cell..
More informationSPINDLE ERROR MOVEMENTS MEASUREMENT ALGORITHM AND A NEW METHOD OF RESULTS ANALYSIS 1. INTRODUCTION
Journal of Machine Engineering, Vol. 15, No.1, 2015 machine tool accuracy, metrology, spindle error motions Krzysztof JEMIELNIAK 1* Jaroslaw CHRZANOWSKI 1 SPINDLE ERROR MOVEMENTS MEASUREMENT ALGORITHM
More informationLecture 4 DISCRETE SUBGROUPS OF THE ISOMETRY GROUP OF THE PLANE AND TILINGS
1 Lecture 4 DISCRETE SUBGROUPS OF THE ISOMETRY GROUP OF THE PLANE AND TILINGS This lecture, just as the previous one, deals with a classification of objects, the original interest in which was perhaps
More informationMath 241 Lines and Planes (Solutions) x = 3 3t. z = 1 t. x = 5 + t. z = 7 + 3t
Math 241 Lines and Planes (Solutions) The equations for planes P 1, P 2 and P are P 1 : x 2y + z = 7 P 2 : x 4y + 5z = 6 P : (x 5) 2(y 6) + (z 7) = 0 The equations for lines L 1, L 2, L, L 4 and L 5 are
More informationTwo vectors are equal if they have the same length and direction. They do not
Vectors define vectors Some physical quantities, such as temperature, length, and mass, can be specified by a single number called a scalar. Other physical quantities, such as force and velocity, must
More informationExplain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds.
Problem 1 Explain the ionic bonds, covalent bonds and metallic bonds and give one example for each type of bonds. Ionic Bonds Two neutral atoms close to each can undergo an ionization process in order
More informationSHAPE, SPACE AND MEASURES
SHPE, SPCE ND MESURES Pupils should be taught to: Understand and use the language and notation associated with reflections, translations and rotations s outcomes, Year 7 pupils should, for example: Use,
More informationChapter 7: Polarization
Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces
More informationDO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS
DO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS Quantum Mechanics or wave mechanics is the best mathematical theory used today to describe and predict the behaviour of particles and waves.
More informationSymmetric Stretch: allows molecule to move through space
BACKGROUND INFORMATION Infrared Spectroscopy Before introducing the subject of IR spectroscopy, we must first review some aspects of the electromagnetic spectrum. The electromagnetic spectrum is composed
More informationPhase transitions with no groupsubgroup relations between the phases
Phase transitions with no groupsubgroup relations between the phases Michele Catti Dipartimento di Scienza dei Materiali, Universita di Milano Bicocca, Milano, Italy International School on the Use and
More informationMath 241, Exam 1 Information.
Math 241, Exam 1 Information. 9/24/12, LC 310, 11:1512:05. Exam 1 will be based on: Sections 12.112.5, 14.114.3. The corresponding assigned homework problems (see http://www.math.sc.edu/ boylan/sccourses/241fa12/241.html)
More information1 The water molecule and hydrogen bonds in water
The Physics and Chemistry of Water 1 The water molecule and hydrogen bonds in water Stoichiometric composition H 2 O the average lifetime of a molecule is 1 ms due to proton exchange (catalysed by acids
More informationUnified Lecture # 4 Vectors
Fall 2005 Unified Lecture # 4 Vectors These notes were written by J. Peraire as a review of vectors for Dynamics 16.07. They have been adapted for Unified Engineering by R. Radovitzky. References [1] Feynmann,
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationSolving Simultaneous Equations and Matrices
Solving Simultaneous Equations and Matrices The following represents a systematic investigation for the steps used to solve two simultaneous linear equations in two unknowns. The motivation for considering
More informationEquations Involving Lines and Planes Standard equations for lines in space
Equations Involving Lines and Planes In this section we will collect various important formulas regarding equations of lines and planes in three dimensional space Reminder regarding notation: any quantity
More informationCopyright 2011 Casa Software Ltd. www.casaxps.com. Centre of Mass
Centre of Mass A central theme in mathematical modelling is that of reducing complex problems to simpler, and hopefully, equivalent problems for which mathematical analysis is possible. The concept of
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationHydrogen Bonds in the Crystal Structure of Strontium Hydroxide Octahydrate Sr(OH) 2 8H 2
Hydrogen Bonds in the Crystal Structure of Strontium Hydroxide Octahydrate Sr(OH) 2 8H 2 O Hans Reuter, Shouassi Kamaha, and Otmane Zerzouf Universität Osnabrück, Institut für Chemie, Barbarastr. 7, D49069
More informationLecture L3  Vectors, Matrices and Coordinate Transformations
S. Widnall 16.07 Dynamics Fall 2009 Lecture notes based on J. Peraire Version 2.0 Lecture L3  Vectors, Matrices and Coordinate Transformations By using vectors and defining appropriate operations between
More informationEarth Sciences: Course Presenters
Earth Sciences: Course Presenters 625102 Geology Dr Stephen Gallagher Prof Andrew Gleadow Dr Malcolm Wallace Prof Ian Plimer Course Coordinator Room 214 Series  Lecture Topics 1. Mineralogy and Crystals
More informationINTRODUCTORY CHEMISTRY Concepts and Critical Thinking
INTRODUCTORY CHEMISTRY Concepts and Critical Thinking Sixth Edition by Charles H. Corwin Chapter 13 Liquids and Solids by Christopher Hamaker 1 Chapter 13 Properties of Liquids Unlike gases, liquids do
More informationarxiv:condmat/0308498v1 [condmat.soft] 25 Aug 2003
1 arxiv:condmat/38498v1 [condmat.soft] 2 Aug 23 Matterwave interference, Josephson oscillation and its disruption in a BoseEinstein condensate on an optical lattice Sadhan K. Adhikari Instituto de
More informationSynthesis and Crystal Structure of Na 2 TiO 3
27 卷 5 期 结 构 化 学 (JIEGOU HUAXUE) Vol. 27, No.5 2008. 5 Chinese J. Struct. Chem. 553~557 Synthesis and Crystal Structure of Na 2 TiO 3 MAO ShaoYu 1 REN XiaoXia ZHOU ZhaoHui (State Key Laboratory for
More informationPiezo Technologies  Technical Resource Paper
in Piezoceramic Materials One can think of a piezoceramic as a rock which generates electrical current if squeezed and which moves if driven by an electrical current. For these wonderful properties to
More informationFURTHER VECTORS (MEI)
Mathematics Revision Guides Further Vectors (MEI) (column notation) Page of MK HOME TUITION Mathematics Revision Guides Level: AS / A Level  MEI OCR MEI: C FURTHER VECTORS (MEI) Version : Date: 97 Mathematics
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS
EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1  LOADING SYSTEMS TUTORIAL 1 NONCONCURRENT COPLANAR FORCE SYSTEMS 1. Be able to determine the effects
More informationME 111: Engineering Drawing
ME 111: Engineering Drawing Lecture # 14 (10/10/2011) Development of Surfaces http://www.iitg.ernet.in/arindam.dey/me111.htm http://www.iitg.ernet.in/rkbc/me111.htm http://shilloi.iitg.ernet.in/~psr/ Indian
More information121 Representations of ThreeDimensional Figures
Connect the dots on the isometric dot paper to represent the edges of the solid. Shade the tops of 121 Representations of ThreeDimensional Figures Use isometric dot paper to sketch each prism. 1. triangular
More informationChapter 22: Electric Flux and Gauss s Law
22.1 ntroduction We have seen in chapter 21 that determining the electric field of a continuous charge distribution can become very complicated for some charge distributions. t would be desirable if we
More information